### IOP Conference Series: Materials Science and Engineering

**PAPER • OPEN ACCESS**

## Considerations on stress triaxiality variation for 2P

## armor steel

**To cite this article: V Zichil et al 2017 IOP Conf. Ser.: Mater. Sci. Eng. 200 012066**

View the article online for updates and enhancements.

### Related content

*Critical Void Volume Fraction fc at Void*
Coalescence for S235JR Steel at Low
Initial Stress Triaxiality

Pawe Grzegorz Kossakowski and Wiktor Wcilik

-Determination of Burst Pressure of API Steel Pipes using Stress Modified Critical Strain Model

N A Alang, N A Razak and A S Sulaiman

-Strain limit dependence on stress triaxiality for pressure vessel steel

Y-C Deng, G Chen, X-F Yang et al.

**1234567890**

Innovative Ideas in Science 2016 IOP Publishing

IOP Conf. Series: Materials Science and Engineering **200**_{ (2017) 012066 doi:10.1088/1757-899X/200/1/012066}

**Considerations on stress triaxiality variation for 2P armor **

**steel **

**V Zichil1, A Coseru2, F Nedeff2 and C Tomozei3**

1

"Vasile Alecsandri" University of Bacau, Department of Economical Engineering, Mechatronics, 600115 Bacau, Romania

2

"Vasile Alecsandri" University of Bacau, PhD student, 600115 Bacau, Romania

3

"Vasile Alecsandri" University of Bacau, Department of Environmental Engineering and Mechanical Engineering, 600115 Bacau, Romania

E-mail: valentinz@ub.ro

**Abstract**. Stress triaxiality is considered an invariant of stress, defined as the ratio of
hydrostatic stress (hydrostatic pressure by other authors) and the equivalent stress (usually
calculated using von Mises criterion). If the values of the main three stresses have comparable
sizes, stress triaxiality can be also calculated using the first invariant of the stress tensor.
Despite that the stress triaxiality is an invariant, the authors have determined experimentally
and analytically its variation with the force at the tensile test, but also with the radius of
notches caused in the specimen. 2P armor steel being used in lightweight armor, these notches
occur after shocks with foreign objects. Furthermore, the authors have revealed the stress
triaxiality variation function of the test type. The tests were performed on tensile specimens
loaded for tensile test, pure torsion test, 25% tensile - 75% torsion test, 50% tensile - 50%
torsion test, 75% tensile - 25% torsion test. The mathematical model used was designed by
Xue.

**1. Introduction **

2P armor steel is used mainly to achieve coatings for armored military vehicles. There are also some special uses, such as fuel pipes for those vehicles [1]. For this reason, a study for 2P armor steel plate and for a limited length tube, in terms of its behavior in plastic domain has to be done.

*1.1. Bridgman's criterion *

Bridgman provides a simple analytical solution to calculate the equivalent stress, using von Mises methodology for the minimum section of a revolution specimen [2].

Bridgman's analysis is applied to revolution specimens (with or without the initial unloading) made
from a homogeneous isotropic material. The material is considered a plastic one (complying Von
Mises plasticity criterion, isotropic hardening and Prandtl-Reuss equations). The specimen is tested to
a tensile force in the direction of its *ez* axis (Figure 1).

Bridgman's specific hypothesis reflects the variation of the curvature radius *ρ* along the *ez* axis. The
proposed mathematical relation has the general form:

2
**1234567890**

Innovative Ideas in Science 2016 IOP Publishing

IOP Conf. Series: Materials Science and Engineering **200**_{ (2017) 012066 doi:10.1088/1757-899X/200/1/012066}

Bridgman had also proposed the maximum triaxiality ratio of stress* τ* (the center of the minimum
sample section), defined by the equation:

### (

### )

(2)where

### -

hydrostatic stress;- equivalent von Mises stress;

- the length of the original ligament; - initial notch radius

*1.*2.* Barsoum – Faleskog’s model*

Barsoum and Faleskog have used a tube with slots in their experiments, as it can be seen in Figure 2
[4]. Their results are reported through the Lode parameter, in reference to *σ1*, *σ2* and *σ3* main stress as a

ratio of the breaking plane, as shown in Figure 3, where Lode’s parameter is defined as:

(3)

*1.3. Xue – Wierzbicki criterion *

Xue și Wierzbicki have shown that the ductile fracture is the result of the accumulation of plastic strain and the damage depends both of the Lode’s angle and hydrostatic pressure. The model used in analytical calculations is represented by a function of the three tensors of the invariant stress:

*J1* – shows the sensitivity of hydrostatic pressure;

*J2* – shows the equivalent von Mises stress;

*J3* – shows the Lode’s angle.

Xue – Wierzbicki criterion suppose that the material is isotope and bears von Mises plasticity criterion, also that the failure is characterized by a deterioration factor formally expressed as (4):

**1234567890**

Innovative Ideas in Science 2016 IOP Publishing

IOP Conf. Series: Materials Science and Engineering **200**_{ (2017) 012066 doi:10.1088/1757-899X/200/1/012066}

**Figure 2. **Notched specimen tube used Barsoum

and Faleskog [4]

**Figure 3. **Specific strains along the main stress

directions [4]

### ( )

(4)where: *σeq,VM* : equivalent von Mises stress ;

*w (D)* : the deterioration factor, D = [0,1].

*1.4. Lode's angle sensitivity *

Lode’s angle is represented in a deviator plane, as the angle between the *O'P* and *O'A* directions,
where *P* is the stress state and *A* is the condition of pure shear (Figure 4) [5].

Lode’s angle is expressed and closely related to the third stress invariant *J3*. Azimuthal dependence

is a function on the Lode’s angle:

**Figure 4. **Lode's angle in a deviator plane

[5]

**Figure 5. ** Graphical representation of the Xue -

4
**1234567890**

Innovative Ideas in Science 2016 IOP Publishing

**200**_{ (2017) 012066 doi:10.1088/1757-899X/200/1/012066}

### ( (

### ))

_{ } (5)

*1.5. Hydrostatic pressure sensitivity *

Stress triaxiality *β* is defined as the ratio between the hydrostatic stress and the equivalent stress:

(6)

where is the equivalent von-Mises stress expressed by:

√

### √(

### )

### (

### )

### (

### )

**(7)**

and *σm* is the hydrostatic stress :

** **(8)

Stress triaxiality (Figure 5) is not constant in the nearest notch, the maximum value is determined behind the crack. Critical effective stress triaxiality is defined as the average value from the stress triaxiality distribution on the effective length.

### ∫

### ( )

_{ }

_{ }_{(9) }

This model involves identifying six material constants: *Plim* – material dependent constant; *q* -

pressure dependent constant; *γ* – Lode’s angle dependent constant; *ξf0* – crack reference strain; *m* -

damage exponent of accumulation; *β* – thinning effect.

**2. Experimental procedure **

A tensile test allows measuring the tensile strength of any material.
This test involves placing a bar of any material between the jaws of a
tensile testing machine to pull the bar until it breaks, according to NF
EN ISO 6892-1: 2009 [7]. As a result of the applied axial force upon
a specimen by the original length (*L0*), a reduction in cross-sectional

area is caused, from *A0* to *A* until the occurrence of breakage. Stress

and length variation between two fixed points is recorded and used to determine the stress-strain state.

Torsion test involves twisting a specimen in the absence of other loads (bending or shear) as is specified in ASTM E143: 2013 [8]. Tests were performed on smooth and notched specimens. The tensile strength was carried out by applying a load force between 10 kN and 25 kN. For different notches, the range of the radius was between 0.5 mm and 10 mm (Figure 6). The same type of specimens was used to analyze the influence and the impact of Lode’s angle and triaxiality. To study the effects of Lode’s angle, smooth specimens have chosen for different tests (pure traction, pure torsion and combined test: tensile 75% - 25% torque, tensile 50% - 50% torque, tensile 25% - 75% torque).

Lode's effectively parameter *ξef* is evaluated based on actual

distance in the middle of the notch. The effective distance *Xef* is given

by the volumetric method [9].

**1234567890**

Innovative Ideas in Science 2016 IOP Publishing

**200**_{ (2017) 012066 doi:10.1088/1757-899X/200/1/012066}

**3. Results **

In order to study the effects of hydrostatic stress, selected notched specimens with the radius of the notch between 0.5 mm and 10 mm were studied.

The value of Lode’s effectively parameter (*ξef*) at pure tensile test is shown in Figure 7. The values

for the radius of the notch and the effective distance (*Xef*) are reported depending on the length of the

notch in Tables 1, 2 and 3.

**Table 3.** Values for *ξef* and *Xef* function of

notch radius at pure traction test σg/σN < 1 ; 100% Traction r [mm] Ξef Xef [mm] 0,5 0,866405 0,68 2 0,816663 0,74 4 0,854189 0,92 10 0,936259 0,98

**Figure 7. ** Lode’s effective parameter variation at pure tensile test

The results of the tests made for combined loads conditions are presented in Figures 8, 9 and 10. As
it may be observed, Lode's parameter values vary between *0* and *1*. A “zero” value corresponds to pure
torsion and the “one” value corresponds to pure traction. Values in the range “zero – one” are for
combination of tensile and torsion load corresponding to different ratios of these two loads.

Preserving at a constant value the triaxiality (pure tensile load on a smooth specimen), Lode’s
parameter can take different values (Lode’s angle varies between *0°* and *30°*). This variation can cause
a significant difference in deformation and also to the material damage, so the material is directly
dependent of Lode’s parameter. This variation can show the influence of the load level. For a higher
tensile load and a reduced torsion load Lode’s parameter is close to the value *1*, which means a small

0.7
0.75
0.8
0.85
0.9
0.95
1
0.5 2 4 10
** ξ**
**ef**
**Notch radius [mm] **

**100 % Pure tensile test **

(Sigma g/ Sigma N) < 1 (Sigma g/ Sigma N) = 1 (Sigma g/ Sigma N) >1

**Table 1.** Values for *ξef* and *Xef* function of

notch radius at pure traction test σg/σN >1 ; 100% Tracțiune r [mm] ξef Xef [mm] 0,5 0,971068 0,64 2 0,944137 0,7 4 0,955766 0,79 10 0,980475 0,88

**Table 2.** Values for *ξef* and *Xef*function of

notch radius at pure traction test σg/σN =1 ; 100% Tracțiune r [mm] ξef Xef [mm] 0,5 0,909574 0,66 2 0,85741 0,72 4 0,907483 0,86 10 0,966831 0,94

6
**1234567890**

Innovative Ideas in Science 2016 IOP Publishing

**200**_{ (2017) 012066 doi:10.1088/1757-899X/200/1/012066}

influence of this parameter. For a higher torsion and a lower tensile load applied, Lode’s parameter is
near *0* values, which means a greater influence of Lode’s parameter.

**Figure 8. ** Lode’s effective parameter variation at 25% tensile – 75% torsion combined test

**Figure 9. ** Lode’s effective parameter variation at 50% tensile – 50% torsion combined test

**Figure 10. ** Lode’s effective parameter variation at 75% tensile – 25% torsion combined test

0
0.1
0.2
0.3
0.4
0.5
0.5 2 4 10
**ξef**
**Notch radius [mm] **

**25% traction -75% torsion test **

(Sigma g/ Sigma N) <1
(Sigma g/ Sigma N) = 1
(Sigma g/ Sigma N) >1
0.5
0.55
0.6
0.65
0.7
0.75
0.8
0.85
0.9
0.5 2 4 10
** ξef**
**Notch radius [mm] **

**50% tensile-50% torsion test **

(Sigma g/ Sigma N) = 1
(Sigma g/ Sigma N) <1
(Sigma g/ Sigma N) >1
0.88
0.9
0.92
0.94
0.96
0.98
1
1.02
0.5 2 4 10
** ξef**
**Notch radius [mm] **

**75% tensile -25% torsion test **

(Sigma g/ Sigma N) <1 (Sigma g/ Sigma N) = 1 (Sigma g/ Sigma N) >1

**1234567890**

Innovative Ideas in Science 2016 IOP Publishing

**200**_{ (2017) 012066 doi:10.1088/1757-899X/200/1/012066}

Contrariwise, the dependence of the Lode’s angle and stress triaxiality (shown in Figure 11 for only one load situation) enables us to make an indirect correlation between the damage risk and the hydrostatic stress.

**Figure 11. ** Triaxiality values and Lode's angle for different notch radius in complex load state:

75% tensile - 25% torsion

**4. Conclusions **

In this paper the authors have proposed to determine stress triaxiality variation on 2P armor steel. Therefor it was determined:

- Stress triaxiality for various types of specimens with different notch radius; - Lode's angle, using the model Xue-Wierzbicki;

- Effective stress triaxiality and effective Lode's angle;

- The influence of stress triaxiality and the influence of Lode angle upon ductile material breakage.

From the analysis of experimental results is easy to observe that stress triaxiality (via Lode's angle) is a very sensitive indicator for material deformation before a ductile fracture. Thus, for 2P armor steel, only at low levels of stress triaxiality the ductile fracture deformation respect the model described in fracture mechanics. At high levels of stress triaxiality (small parameter values for Lode's) a breakage of the material can occur suddenly. Therefore, the authors believe that the introduction of Lode’s parameter as a new indicator in the model of ductile fracture is required. Lode's parameter can be associated with the breakage material characteristics.

**References **

[1] ***https://www.4tuning.ro/ghidul-soferului/ce-presupune-o-masina-blindata-care-sa-faca-fata-unui-atac-terorist-28474.html

[2] Bridgman P 1944 The Stress Distribution at the Neck of a Tension Specimen, *Trans. ASME***32 **

553-574

[3] Valiente A 2001 On Bridgman’s Stress Solution for a Tensile Neck Applied to axisymmetrical
Blunt Notched Tension Bars, *Journal of Applied Mechanics***68** 412-419

[4] Barsoum I and Faleskog J 2007 Rupture mechanisms in combined tension and shear –
Experiments, *International Journal of Solids and Structures***44** 1768-1786

[5] Xue L 2007 *Ductile fracture modeling – theory, experimental investigation and numerical *
*verification*, Massachusetts Institute of Technology, Doctoral Thesis

[6] Xue L and Wierzbicki T 2008 Ductile fracture initiation and propagation modeling using

r=0,5 mm
r=2 mm
r=4 mm
r=10 mm
0.92
0.93
0.94
0.95
0.96
0.97
0.98
0.99
1
1.01
0.4 0.45 0.5 0.55 0.6 0.65
**ξef**
**Triaxiality β _{ef }**

**75% tensile-25% torsion test **

(Sigma g/Sigma N)<1 (Sigma g/Sigma N)=1 (Sigma g/Sigma N)>1

8
**1234567890**

Innovative Ideas in Science 2016 IOP Publishing

**200**_{ (2017) 012066 doi:10.1088/1757-899X/200/1/012066}

damage plasticity theory, *Engineering Fracture Mechanics***75** 3276-3293

[7] ***Norme NF EN ISO 6892-1: 2009, *Matériaux métalliques - Essai de traction - Partie 1* :
méthode d'essai à température ambiante

[8] ***ASTM E-143: 2013, *Standard Test Method for Shear Modulus at Ambient Temperature*

[9] Pluvinage G 2007 *General approaches of pipeline defect assessment in Safety Reliability and *
*Risks associated with water, oil and Gas pipelines*, Edited by Pluvinage G and Elwany M ,
Springer